Photoassisted Scanning Tunneling Microscopy and Tunneling ...bard.cm. · PDF file...
Embed Size (px)
Transcript of Photoassisted Scanning Tunneling Microscopy and Tunneling ...bard.cm. · PDF file...
J. Phys. Chem. 1993,97, 1431-1436 1431
Photoassisted Scanning Tunneling Microscopy and Tunneling Spectroscopy of n-Type Tungsten Diselenide (n- WSe2) Single Crystals
Fu-Ren F. Fan and AUen J. Bard’ Department of Chemistry and Biochemistry, The University of Texas at Austin, Austin, Texas 7871 2
Received: August 14, 1992; In Final Form: November 4, 1992
The van der Waals surface (perpendicular to the c axis) of a nondegenerate n-type WSe2 single crystal was imaged at negative substrate bias voltage (V) in the constant-current mode in air with a scanning tunneling microscope (STM) combined with optical excitation techniques. A current (i) image at a positive bias under steady-state illumination, obtained simultaneously with the topographic image, revealed that the photocurrent a t the step edges was much smaller than that in the defect-free region. This reduction of the photocurrent a t defect sites is attributed to a high surface recombination rate a t defects. Tunneling spectroscopy (TS) performed in Nz, including i vs V and di/dVvs Vcurves with the tip held over the n-WSe2 surface, was also carried out both in the dark and under laser irradiation. The results were interpreted in terms of the band locations and minority carrier injection through photoexcitation.
Transition-metal dichalcogenides have been used as semicon- ductor electrodes in photoelectrochemical (PEC) cells.] The behavior and efficiencies of these cells depend strongly on the natureof the electrode surface.2” Scatter in the electrochemical (EC) parameters and the PEC behavior found in such cells by different laboratories can be attributed to significant sample- to-sample variations in the morphology of the WSe2 crystals employed as electrodes. For example, the presence of exposed edges on the van der Waals surface leads to significant dark anodic currents at n-type electrodes and lower photocurrent e f f i c i en~ ies .~~*~~ Thus, methods of examining the surface to characterize defects on semiconductors exposed to gaseous or liquid environments, and especially techniques capable of high spatial resolution, are very useful. For example, Parkinson and co-workers’ have successfully used a scanning laser system in a PEC cell to identify semiconductor surface topological features and to correlate these features to the carrier collection efficiency. The scanning tunneling microscope (STM)8 can also be used in measurements of irradiated semiconductor surfaces by combining STM with optical technique^.^ This new method can provide spectroscopic information about the surface and near-surface region with high spatial resolution.
Since cleaved surfaces of WSe2 are atomically flat and inert tooxidation, this semiconductor is especially suitable for tunneling microscopy experiments.lWl4 Akari et a1.I0 recently reported preliminary results on the photoaction spectra of p-WSe2 with an STM. Information about energy-dependent creation and recombination of charge carriers in the vicinity of the surface can be obtained by photoassisted tunneling spectroscopy (PATS) without the necessity of covering the surface with a conducting film.
In this paper, as an extension of our STM and tunneling spectroscopy (TS) studies on n-TiO2 (001)15a and n-FeS2 (001) surfaces,Isb we report a series of experiments involving TS measurements of a tunnel junction consisting of a metal tip and an n-WSe2 substrate in the dark and under laser irradiation. The differential conductance spectra obtained in the dark and under illumination are compared. The light-induced excess (photo) current was found tovary spatially, with largedecreases occurring at step edges where there are higher rates of recombination of the charge carriers. The short-circuit photocurrent ( i X ) and open- circuit voltage (V,) (under laser irradiation) depended on the distance between the tip and the substrate.
0022-3654/93/2097-143 1 %04.00/0
The n-WSe2 single crystals were grown by the vapor-transport method.16 The resistivities of the crystals ranged from 0.1 to 0.2 il cm. To prepare fresh WSe2 surfaces, the top layers of the bulk crystals were peeled off with adhesive tape in the air. The thin WSe2 layers used in the back-illumination experiments were prepared by peeling them off of a bulk crystal with tape, which was then removed from the thin layer by dissolving the tape in methylene chloride. The optical transmission of these thin WSez layers at 632.8 nm ranged from 1% to 10% (corresponding to thicknesses of ca. 0.1-0.2 ~ m ) . ~ ’ Ohmic contacts were made by rubbing In-Ga alloy on the outside edges of the crystal. An electrical lead was then connected to the contact with conductive silver paint (Acme Chemicals & Insulation Co., Allied Products Corp., New Haven, CT). The electrode was covered, along with the contact and all sides of the crystal, except for an exposed area of ca. 0.01 cm2, on the surface with insulating epoxy. The electrodes studied here showed mirrorlike surfaces with no obvious edges and pits on the surfaces when examined at a magnification of 200x.
The STM apparatus and the detailed procedures for current and differential conductance measurements have been described previ0us1y.l~ Briefly, current images (constant height) were obtained by stabilizing the feedback loop at a bias voltage of -1 .O V (in all cases reported, bias is that of the substrate vs tip) and with a reference current of 0.1 nA and then interrupting the feedback loop and measuring the tip current at the desired bias at each location. In TS measurements, after interruption of the feedback loop, the bias voltage (V) was swept linearly at ca. 2 V/s and the current ( i ) was recorded to obtain the i-Vcurve. A 10-20-mV peak-to-peak sinusoidal signal (AV) at 10 kHz was superimposed on the dc ramp, and the variation in the in-phase current (Ai) was determined with a lock-in amplifier to obtain the differential conductance, di/dV, as a function of V. All conductances reported here represent the differential conductance, unless otherwise indicated.
Electrochemically etched Ir-Pt tips (FHC Co., Brunswick, ME) were employed. All experiments, unless indicated otherwise, were performed under Nz, either in the dark or under irradiation with an 8 mW He-Ne laser (Spectra-Physics Inc., Mountain View, CA). The experiments in Nz were performed by keeping the STM unit in a machined Plexiglas chamber, which was continuously purged with purified Nz.
Q 1993 American Chemical Society
1432 The Journal of Physical Chemistry, Vol. 97, No. 7, 1993
Current-Voltage Curves b-m rUD>
Fan and Bard
Gap (-0.1 V, 0.5 nA) \
lyGap (-1.0 V, 0.5 nA) ‘q
6 - k 0 a 0-
-2 -1 0 1 I
w- n UP). V Figure 1. Current vs voltage curves in the dark for an Ir-Pt tip and an n-WSe2 sample at various tipsample separations. 1: reference t i p sample separation (SO) defined by a current 0.5 nA at bias voltage -1.0 V. 2: SO -5 A. 3: SO -10 A. 4: SI for i = 0.5 nA and V = -0.1 V.
Result9 Current-Voltage Relation in the Dark. In Figure 1, the
experimentally determined i-Vrelationships in the darkat various tipsubstrate separations, s, are shown. Since the absolute value of the tipsubstrate gap cannot be determined, a relative separation, at a designated reference current and bias voltage, was arbitrarily taken as the reference gap [e.g., SO for i = 0.5 nA at V=-l.OV(curve l )andsl fori=O.SnAat V=-0.1 V(curve 4)], and other distances are given with respect to this gap. As shown in this figure, the magnitude of the current at a given bias strongly depends on s. At a givens, the current depends strongly on the bias voltage, and the i-V curves display very asymmetric (Schottky diodelike) behavior. Note that for a given voltage magnitude, the current is much larger at negative bias than at positive bias. In the negatively biased voltage region, at large s (curves 1 and 2), the i-Vcurves were not smooth and showed several shoulders near -1.5 V. As s decreased, the i-V curves bccame fairly smooth and approached a nearly exponential dependence at large bias (curve 4). In the positive-bias region, essentially no current could be detected when s was large (curves 1 and 2), while at smaller gaps significant current was observed when the bias was greater than 0.5 V (curves 3 and 4). The magnitude of the current in this region, as compared with the i-V curves in the negative-bias region, was less dependent on s.
ConductmnceVoltage Relation in the Dark. Figure 2 shows thedifferentialconductance (di/dV) spectra over the bias voltage range of -1 .5 to + 1.7 V for two different gap separations (SO and sI). At the larger gap (SO), thedifferential conductance wasvery low in the positive-bias region (curve 1). In the negative-bias region, the di/dV spectrum showed a peak near -1.4 V where a shoulder was observed in the i-Vcurves. At the smaller gap, sI, the differential conductance in the positive-bias region was greatly enhanced. As shown in curve 2, two well-defined peaks can be identified: a prominent symmetric peak with a half-height width of ca. 0.2 eV at ca. 0.8 V and a broader peak located at ca. 1.5 V. Following this broad peak, the differential conductance increases again with increasing bias. In the negative-bias region, high differential conductance was observed even at the larger distance.
Current-Voltage Relation under Irradiation. Figure 3 shows two i-V curves at a gap defined by -1.0 V and 0.28 nA, one in the dark and the other under front surface ill